Writhe and mutual entanglement combine to give the entanglement length E. Panagiotou,1,* M. Kr¨oger,2,† and K. C. Millett1 1

Department of Mathematics, University of California, Santa Barbara, California 93106, USA 2 Polymer Physics, Department of Materials, ETH Zurich, CH–8093 Zurich, Switzerland (Received 23 May 2013; revised manuscript received 25 September 2013; published 30 December 2013) We propose a method to estimate Ne , the entanglement length, that incorporates both local and global topological characteristics of chains in a melt under equilibrium conditions. This estimate uses the writhe of the chains, the writhe of the primitive paths, and the number of kinks in the chains in a melt. An advantage of this method is that it works for both linear and ring chains, works under all periodic boundary conditions, does not require knowing the contour length of the primitive paths, and does not rely on a smooth set of data. We apply this method to linear finitely extendable nonlinear elastic chains and we observe that our estimates are consistent with those from other studies. DOI: 10.1103/PhysRevE.88.062604

PACS number(s): 83.80.Sg, 02.10.Kn, 83.10.Kn, 05.40.Fb

I. INTRODUCTION

The rheological properties of polymer melts are determined primarily by the random-walk-like structure of the constituent chains and the fact that the chains cannot cross [1]. The motion of sufficiently long chains is limited by the presence of the other chains which create persistent obstacles, called entanglements [2]. As the degree of polymerization becomes larger than the entanglement length, Ne , the entanglements become important and dramatically change many melt properties such as diffusivity and viscosity. In entangled polymer melts and solutions, Ne is arguably the most fundamental material parameter which can be measured experimentally by the plateau modulus [3]. Edwards suggested that entanglements effectively restrict individual chain conformations to a curvilinear tubelike region enclosing each chain [1]. For very short time scales, chain segments are allowed to freely fluctuate in all directions until their displacements become commensurate with the tube diameter, a, which is related to entanglement length by a 2 = Ne b, where b is the bond length [4–6]. Thus, Ne characterizes the crossover between the Rouse and the reptation regime and it is commonly interpreted as the number of monomers between entanglements. The axis of the tube is a coarse-grained representation of the chain, called the primitive path (PP). Edwards defined the PP as the shortest path a chain, fixed at its ends, can follow without crossing any other chains. Based on this definition, Rubinstein and Helfand [2] realized that the entanglements in a system could be obtained by reducing all chains to their PPs simultaneously, creating a PP network. Since then several methods have been developed for extracting the PP network [7–13]. Two geometrical methods capable of efficiently reducing computer generated polymer models to entanglement networks are the Z1 code [8,9,14,15] and the CReTA algorithm [10]. All the methods work in discontinuous coordinate space; i.e., they use finite displacements during which disentanglement events must be avoided. Despite differences in their specific implementation, these methods are reported to yield similar

* †

Corresponding author: [email protected] http://www.complexfluids.ethz.ch

1539-3755/2013/88(6)/062604(17)

results for the average properties of the PP network [9]. These algorithms extract the PP network estimate of Ne either from the chain statistics of the PPs or from direct enumeration of entanglements, defined as contacts between PPs. The different approaches produce somewhat different results for Ne for the same atomistic configurations [6,9,10,16,17]. Indeed, the resulting PP network is not unique and several of its features, such as the role of self-entanglement, the difference between energy minimization and length minimization, and the location of entanglement points along a PP, have been examined [8–10,18–22]. Notice that the process of drawing the strands tight destroys the detailed geometry of the melt and these methods may lead one to think of entanglements as local binary contacts between two chains. To better capture the geometry, other methods to extract the PP such as the time isoconfigurational average [23–25] have been proposed. Despite these advances, our understanding of entanglement is incomplete. The reason is the difficulty to connect the entanglement properties of the chains at two different scales. In the rest of this paper we shall call the local obstacles to the motion of the chains local entanglement, and we shall call the conformational complexity of the entire conformations of the chains in the melt global entanglement (see Fig. 1 for an illustrative example). Edwards first pointed out that in the case of ring polymers, the global entanglement of the chains can be studied by using tools from mathematical topology, such as the Gauss linking number [26,27]. First, notice that the uncrossability of the chains allows them to attain only isotopic configurations, that is, configurations that are related by continuous deformations that do not allow intersections. This notion of isotopy is a basic concept in topology. Under certain conditions, we can model the polymer chains as simple mathematical curves in space. A knot (respectively, link) is one (or more, respectively) simple closed curve(s) in space without intersections. The complexity (or topological state) of these knots or links is related to their global entanglement and it can be measured by using topological invariants such as knot or link polynomials [28–31]. The topological invariants are properties of knots or links, which are the same for isotopic configurations. Since Edwards, many studies have been devoted to the topology of polymer rings and its relation to physical properties [7,32–35]. The study of global entanglement has been very useful, especially in the study of

062604-1

©2013 American Physical Society

¨ E. PANAGIOTOU, M. KROGER, AND K. C. MILLETT

PHYSICAL REVIEW E 88, 062604 (2013)

FIG. 1. (Color online) Example of two conformations with the same number of kinks, Z = 6, but with different writhe, W = 0.007 (left) and W = 2.78 (right). We notice that the conformation of the former chain is simple, while the latter is more complex. A direct end-to-end closure of the first chain will produce the unknot (the trivial knot type), while the direct end-to-end closure of the second results in the trefoil knot (a nontrivial knot type). Notice that the disentanglement of the second conformation may be difficult [69].

biopolymers [36,37]. In Ref. [34] a direct relation between distinct topological states and Ne has been revealed. Therein, Ne was estimated for a system of ring polymers in one or two PBC, using purely topological tools, i.e., the Jones and the HOMFLY polynomials [28,30,34]. One of the reasons why this has not been explored as much in the case of polymer melts is because of the problem of dealing with linear polymers. In the case of linear polymers, the notion of topological invariant does not apply since topological open curves can be continuously deformed to attain any configuration. Efforts have been made to characterize the knotting of an open chain [33,38–40]. For example, one can use the methods described in Refs. [39,40] to determine the spectrum of knotting arising from the distribution of knot types created by closure of the open chain to the “sphere at infinity.” In this study we will measure the global entanglement of open chains directly without employing any closure. Our goal is to provide a method to estimate Ne for a melt of both linear or ring polymers in any PBC model by combining the local and global entanglement characteristics of the chains in a melt. A measure of global entanglement, that is meaningful both for closed or open chains, is the Gauss linking integral. For two closed chains (ring polymers) the Gauss linking integral is a topological invariant that measures the algebraic number of times one chain turns around the other. For two open chains (linear polymers), it is a real number that is a continuous function of the chain coordinates. The Gauss linking integral can be also applied to one chain in order to provide a measure of global self-entanglement of a chain, called the writhe [41–46]. The writhe is a real number that changes continuously under continuous deformations of a chain. The writhe is very clearly not a topological invariant, even for closed chains, because it is a quantity that depends on

the specific geometry of the chain, and it is very sensitive to the specific conformations that are analyzed. Computer experiments indicate that the linking number and the writhe are effective indirect measures of global entanglement in systems of random filaments [26,32,35,47–55]. Analytical and numerical results have shown that the writhe of random walks and polygons depends on their length and that it follows a different scaling for random walks in a lattice or under confinement [42,53,56–67]. Kholodenko and Vilgis [68] have proved that the writhe of semiflexible rings follows a scaling that depends both on the stiffness parameter and on the length of the chains. The information provided by the writhe is very useful but it is not clear how to put it into the context of current tube and slip-link model methods [69]. In this paper we show that the writhe in combination with the Z1 algorithm can provide information that is relevant to the physical notions of entanglement, such as Ne estimators, denoted Ne (N), that aim at estimating Ne = limN→∞ Ne (N ) from information derived from a finite number of monomers per chain, N . The paper is organized as follows: In Sec. II we describe the measures of entanglement that are used in this paper. In Sec. II B1 we numerically study the mean absolute writhe of semiflexible linear chains in order to extend the analytical result of Kholodenko and Vilgis [68] to open chains. We will use this in the following section in order to estimate Ne for linear chains in a melt. In Sec. III an Ne estimator is introduced based on the writhe of the original chains, the writhe of their PPs, and the number of kinks. In Sec. IV we compute the proposed Ne estimator for linear, finitely extendible nonlinear elastic (FENE) chains in a melt and compare it with the results of previous estimators for the same system. Next, in Sec. V, we discuss some results stemming from the earlier analysis concerning the number of kinks, the writhe of the original chains, the writhe of their PPs, and the writhe of the entanglement strands. These provide further insight to the global and local entanglement of the system. II. MEASURES OF ENTANGLEMENT OF A LINEAR POLYMER CHAIN IN A MELT

To measure the entanglement of polymer chains in a melt we measure their writhe and use the Z1 algorithm to determine their PP. This section is devoted to their description. A. Z1 algorithm

The Z1 algorithm [14] is a state-of-the-art geometric algorithm which proceeds by transforming the physical picture of topological interchain constraints (as conceived by DoiEdwards [1]) into a pure mathematical problem of identifying the shortest multiple disconnected (primitive) path subject to geometrical constraints arising from the configuration of the corresponding atomistic system. More precisely, given a fixed polymer melt configuration, the algorithm minimizes the contour length of the chains by moving the beads sequentially in space, maintaining the noncrossability of the chains. In this way the chains become rectilinear strands coming together at kinks where the entanglements occur. Disentanglement is prevented by constraining moves of kinks to lie in the

062604-2

WRITHE AND MUTUAL ENTANGLEMENT COMBINE TO . . .

plane of their adjacent segments. The Z1 code provides the option to respect or neglect self-entanglements, that is, kinks between arcs of the same chain. Computational effort is, in both cases, very comparable. For a system of M chains of N monomers each, the computational effort of the Z1 algorithm is of the order M N , i.e., almost linear in the total number of monomers [8]. In previous studies it has been shown that self-entanglements between distant chain sections in polymer melts are rare [18]. In this study, to allow for a direct comparison with previous works [17], we use the version of Z1 that does not capture self-entanglements. We stress that, even if there are no kinks of a chain with itself, this does not mean that a chain is not entangled with itself at a global level. This global self-entanglement is imposed to a chain due to the presence of the other chains (see Fig. 1 for an illustrative example). Thus, even if self-crossings are allowed, on average the global self-entanglement remains due to the uncrossability with other chains. A direct consequence of the specific mathematical formulation is that the Z1 algorithm provides as output the average contour length of a primitive path, Lpp . Here and in the following, denotes averaging over all chains of a given configuration. In addition, by mapping the extracted interior nodes of each primitive path into kinks, the average number of interior kinks (entanglements), Z, per chain is returned. The probability distribution of Z has been approximated by a Poissonean [19,70] (Appendix D). We will use the following notation for the average values of these quantities over all chains: Z = Z and Lpp = Lpp . Finally, from the output of Z1 one can recover Ne values in accordance with experiments [17] (Sec. IV A). B. The writhe of a curve

Consider a frozen configuration of polymer chains represented by a collection of polygonal curves in three-dimensional space. A simple measure of global self-entanglement for individual chains is given by counting the crossings in a random projection of one or two chains. Indeed, notice that in all generic orthogonal projections of a planar curve one would not see any crossings. Similarly, for two unlinked planar curves, almost all projections would give no crossings between them. Without loss of generality, we can assign an orientation to the chains. By assigning a sign to each crossing (Fig. 2), one can recover information concerning which arc passes over and under the other. To appreciate the character of the writhe

FIG. 2. (a) +1 crossing and (b) −1 crossing. By assigning a sign to each crossing, one recovers information concerning which arc comes over and under.

PHYSICAL REVIEW E 88, 062604 (2013)

of a chain we first introduce a linking number. We follow the presentation in Ref. [66]. For a generic projection of two oriented curves l1 , l2 to a plane defined by a vector ξ ∈ S 2 the linking number of a diagram, denoted lkξ (l1 ,l2 ), is equal to one half the algebraic sum of crossings between the projected curves. The linking number of two oriented curves is then equal to the average linking number of a diagram over all possible projection directions, i.e., L(l1 ,l2 ) = (4π )−1 ξ ∈S 2 lkξ (l1 ,l2 )dS. This can also be expressed by the Gauss linking integral for two oriented curves. The Gauss linking number of two oriented curves l1 and l2 , whose arc-length parametrization is γ1 (t),γ2 (s), respectively, is defined as a double integral over l1 and l2 [71] as follows: (γ˙1 (t),γ˙2 (s),γ1 (t) − γ2 (s)) 1 L(l1 ,l2 ) = dtds, 4π [0,1] [0,1] |γ1 (t) − γ2 (s)|3 (1) where the nominator of the integrand is the triple product of γ˙1 (t),γ˙2 (s), and γ1 (t) − γ2 (s). Similarly, for the generic orthogonal projection of one oriented curve l to a plane defined by a vector ξ ∈ S 2 we define the writhe of a diagram, denoted wξ (l), to be equal to the algebraic sum of crossings of the projection of the curve with itself. Then the writhe of a curve is defined as the average writhe of a diagram of the curve over all possible projections, i.e., W (l) = (4π )−1 ξ ∈S 2 wξ (l)dS. Analogously, this can be expressed as the Gauss linking integral over one curve. The writhe of an oriented curve l with arc-length parametrization γ (t) is thus alternatively and more conveniently defined by the Gauss linking integral over a curve, (γ˙ (t),γ˙ (s),γ (t) − γ (s)) 1 W (l) = dtds, (2) 2π [0,1]∗ [0,1]∗ |γ (t) − γ (s)|3 where [0,1]∗ × [0,1]∗ = {(x,y) ∈ [0,1] × [0,1]|x = y}. We observe that the geometrical meaning of the writhe and the linking number is the same for open or closed curves, and it is the average over all projection directions of the algebraic sum of crossings, or intercrossings, respectively, in the projection of the curve, or curves, respectively. When applied to open chains both measures are continuous functions in the space of configurations. Furthermore, as the end points of the curves move towards coincidence, the linking number or writhe tends to the values of those measures for the resulting closed knots or links. In the case of closed chains the linking number is a topological invariant. For a polygonal curve the Gauss linking integral can be easily computed following the algorithm described in Ref. [43]. More precisely, for a system of M chains of N monomers each, the computation of the writhe for all chains is of the order M N(N − 1)/2. It has been shown numerically that the writhe follows a normal distribution [65], centered around zero. For a system of many chains in a simulation box, and a large sample, the statistics of the writhe could be estimated from a subset of the chains in each polymer melt configuration. If only a fraction ∼1/N of all chains (requiring M N ) is sufficient to estimate the writhe, the computational effort is of the order of the Z1 code M N .

062604-3

¨ E. PANAGIOTOU, M. KROGER, AND K. C. MILLETT

PHYSICAL REVIEW E 88, 062604 (2013) 6 5

4 3

κ = 0.8 κ=1 κ=2 κ=5 κ = 10 κ = 20 1/2

0.30N

− 0.43

50

100

2 1

(a)

0 0

6 5 4

In the following we will take averages of the writhe of polymer chains in melts simulated with the use of a periodic box. The periodic box is replicated in space to form a large bulk system. As it has been pointed out in previous studies [34,72,73], the periodicity of the chains induces special features in the global entanglement of the melt. For a system with M chains in a periodic box, there are only M different conformations in the periodic system that the box generates and infinitely many copies of these conformations. In this study we will use the writhe to measure the global self-entanglement characteristics per chain in the periodic system. Thus, for a system of M chains in a periodic box it suffices to measure the writhe of the M different unfoldings in order to measure the average writhe per chain in the periodic system. Notice that the average writhe over the space of possible configurations is zero since it can take positive or negative values with the same probability. This is why we choose to study the mean absolute or the mean-squared writhe in the space of configurations. The growth rate of the mean absolute writhe of (open) self-avoiding random lattice walks is equal to that of (closed) self-avoiding √ random lattice polygons [64,65]. Both writhes scale as ∼ N with chain length N . The mean-squared writhe of (closed) equilateral random polygons in three dimensions scales as ∼N [67]. In this paper we will be interested in the scaling of the mean absolute and the mean-squared writhe of linear FENE chains in a melt, for which reference results do not exist. Chains in melts are expected to behave like ideal chains due to screening, and as N → ∞, the known random-walk models are expected to give similar qualitative results for the mean absolute and the mean-squared writhe. We are, however, interested in the precise determination of the involved constants and prefactors of these scalings.

3

150 N

200

250

300

200

250

300

κ = 0.8 κ=1 κ=2 κ=5 κ = 10 κ = 20 (1/4)[(N/κ)1/2 + (κ/N)1/2 − 2]

2 1

(b)

0 0

50

100

150 N/κ

1. The writhe of semiflexible linear chains

Individual polymer chains in a melt are essentially semiflexible, that is, they assume conformations similar to those of wormlike chains with a bending angle constraint imposed (see Appendix A). The main source of semiflexibility are the excluded volume interactions between adjacent monomers. Thus, the writhe of semiflexible chains may provide useful information for the writhe of polymer chains in a melt. Kholodenko and Vilgis [68] provided an analytic expression for the behavior of the mean-squared writhe of linear semiflexible rings as a function of their stiffness parameter. Based on our numerical results, presented below, we will extend their result to linear semiflexible chains and, at the same time, to linear polymer chains in a melt. To compare these results with those for random walks we will also numerically study the mean absolute and the mean-squared writhe of equilateral random walks. Consider a wormlike chain (WLC), a connected linear string of N − 1 segment unit vectors with dimensionless stiffness parameter κ (Appendix A). Kholodenko and Vilgis [68] proved that, for semiflexible rings, the mean absolute writhe behaves as 1/2 −1/2 N π N , (3) |W | = + const 2 κ κ with an unspecified constant.

FIG. 3. (Color online) (a) Numerical results for the mean absolute writhe vs N for various stiffness parameters κ. We include the result for an equilateral random walk, Eq. (6). (b) The same data vs N/κ falls onto a master curve, our Eq. (4).

By generating linear semiflexible chains of varying κ for a range of molecular weights (Appendix A), we find that |W | is a universal function of N/κ (Fig. 3). A best fit for linear chains turns out to be of a form very similar to the one proposed for semiflexible rings, Eq. (3). We find 1/2 −1/2 N N 1 π + −2 . (4) |W | ≈ 5 2 κ κ The difference, compared with the result for rings, is that we have a constant offset and a different prefactor. Our expression implies |W | = 0 for κ = N . The first term in Eq. √ (4) dominates the typical case of N κ. Notice that 1/5 π/2 ≈ 1/4. For any N , the mean absolute writhe of the linear semiflexible chains is smaller than that of rings. Indeed, previous studies on the average crossing number of equilateral random walks and polygons [42,74], on the writhe, on the self-linking number of uniform random walks and polygons in confined space [66,75], and on the writhe of self-avoiding walks or polygons on a lattice [64,65], indicate that the growth rate of these quantities is the same for open and closed chains

062604-4

WRITHE AND MUTUAL ENTANGLEMENT COMBINE TO . . . 35 30

20

2

25

PHYSICAL REVIEW E 88, 062604 (2013) III. A METHOD TO COMPUTE Ne ESTIMATORS VIA WRITHE AND Z

κ = 0.8 κ=1 κ=2 κ=5 κ = 10 κ = 20

In this section we study the number of monomers in an entanglement strand and suggest an Ne estimator for polymer chains in a melt. To do this, we will combine the local entanglement information, provided by the Z1 algorithm, on the number of kinks per chain with the global entanglement information given by the writhe of a chain and its primitive path.

1.18

0.03(N/κ)

15 10

A. Ne via writhe and Z 5 0 0

100

200 N/κ

300

Let us consider a polymer chain, I , in a melt formed by Z + 1 entanglement strands denoted as e1 , e2 ,..., eZ+1 . The writhe of I can be expressed as (Appendix B)

400

FIG. 4. (Color online) Numerical results for the squared writhe vs N/κ for various N and stiffness parameters κ. The data fall onto a master curve, see our Eq. (5).

but with different constants and prefactors. Similarly, shape descriptors such as the radius of gyration, the asphericity, or prolateness also differ for open and closed chains of the same length [76,77]. Similarly, we find that W 2 (Fig. 4) is very well approximated by 1.18 N 2 W ≈ 0.03 . (5) κ Semiflexible chains are ideal in the sense that they behave like random walks of a different step size than that of the bond length. This quantity is called the Kuhn length. It is therefore natural to compare our data with that of random walks that exhibit a fixed edge length and no bond angle correlation. Numerical and analytical arguments show that the mean-squared writhe of closed equilateral random polygons is well described by 0.1334 N − 0.7554 [67]. Here, we extend this analysis to open chains. To generate equilateral random walks, each edge vector was drawn from a uniform distribution on S 2 . Each data point is an average of 5000 random walks. Our numerical results on the mean absolute and the mean-squared writhe, respectively, of equilateral random walks are well described by the following expressions: |WRW | ≈ 0.29 N 1/2 − 0.43, 2

WRW ≈ 0.11 N − 0.95,

W (I ) =

Z+1

W (ei ) + 2

i=1

Z Z+1

L(ei ,ej ),

(7)

i=1 j =i+1

where W (ei ) denotes the writhe of the entanglement strand ei and L(ei ,ej ) denotes the Gauss linking number for entanglement strands i and j . We now focus on the second summation in the right side of Eq. (7). Each term in that summation is a linking number between two entanglement strands of I . The linking number of two polymer chains before and after the application of a reduction algorithm is approximately the same [72]. Notice that the entanglement strands are polymer chains themselves. So, letting r(ei ) denote the strand ei after the reduction, we use the following approximation (see the examples in Fig. 5), L(ei ,ej ) ≈ L(r(ei ),r(ej )).

(8)

Notice that this approximation is valid even if the selfentanglements within an entanglement strand are neglected. Notice next that, by definition, r(ei ) must be a straight rod, and it is an edge of the primitive path that corresponds to I , PP(I ). Further, by definition, the writhe of PP(I ) is given by W (PP(I )) = 2

Z Z+1

L(r(ei ),r(ej )).

(9)

i=1 j =i+1

(6)

which can be derived from Eq. (4) for κ ≈ 1/2. We remind the reader that Eqs. (4)–(6) are not analytical results. However, the best fit of Eq. (4) is based on the analytic formula of Eq. (3) for semiflexible rings [68], and Eq. (6) is also based on semianalytical arguments for random walks [64,65,67]. The exponent in Eq. (4) is only an apparent exponent. If analytical arguments provide exact estimates of those functions in the future, these could be substituted in the following analysis to provide more accurate numerical results. The current estimates are sufficient for testing the proposed methods in this study.

FIG. 5. (Color online) (a) Let e1 ,e2 be two entanglement strands [the black and gray (cyan) curves respectively]. Their Gauss linking integral is L(e1 ,e2 ) = −0.166 667. (b) Let r(e1 ),r(e2 ) denote the corresponding reduced chains. Notice that these are the edges of the PP. Their Gauss linking integral then is L(e1 ,e2 ) = −0.165 372.

062604-5

¨ E. PANAGIOTOU, M. KROGER, AND K. C. MILLETT

PHYSICAL REVIEW E 88, 062604 (2013)

Based on these observations, by Eqs. (8) and (9), we use the following approximation in the rest of this paper: W (PP(I )) ≈ 2 L(ei ,ej ). (10) i 30. Since the variance of Z is of the same order as Z [19,70], the error mean of Z, erZ , of a sample polymer melt √ of C independent √ configurations is erZ = Z/C ≈ 0.1 N/C. Thus, for our systems of N < 400 (C > 100), we obtain erZ < 0.2, which is small compared with the values of Z. Figure 11 shows the data of Fig. 7(a) in double logarithmic representation. We clearly observe a crossover at about N ≈ 45 where Z ≈ 2. This may indicate that chains of N < 45 are only weakly entangled and that the value Z = 2 serves to mark the transition to the asymptotic linear behavior. Figure 7(b) shows the average contour length Lpp of the PP that increases linearly with N , in agreement with earlier works [17]. B. The writhe of linear FENE chains in a melt

In Sec. II B1 we show that the mean absolute writhe of semiflexible chains of length N and stiffness κ can be 1 0.5 0 〈Z〉

200 N

−0.5

10

100

In Fig. 7(a) the value of Z is shown for various chain lengths N . Our result is in agreement with previous studies which predict a linear scaling of Z with N [8,9]. A linear fit of our N > 40 data yields

log

0 0

−1 −1.5 fit to N < 45 fit to N > 45 log10〈 Z 〉

−2 −2.5 1

1.5

2 log10 N

2.5

3

FIG. 11. (Color online) Average number of kinks per chain with the length of the chains in double-logarithmic representation reveals a crossover at N ≈ 45 that finds its analog in the writhe of the PPs.

062604-9

¨ E. PANAGIOTOU, M. KROGER, AND K. C. MILLETT

10

0

〈 |WRW| 〉 Eq. (26)

3 2.5

−2

−3

6

〈 |W| 〉 Eq. (27)

−1

−4

1

2 Log(N)

〈 |W| 〉

〈 |W| 〉

8

3.5

1

〈 |W| 〉 〈 |WPP| 〉 Log(〈 |W| 〉)

12

PHYSICAL REVIEW E 88, 062604 (2013)

3

2 1.5

4 1

2

(a)

0.5

0 0 70

100

200 N

RW

〉

Eq. (28)

0 2

〈 W2

Log(〈 W 〉)

50

2

−1 −2

〈 W2 〉

−3

40

−4 −5

30

1

2 Log(N)

3

20 10

(b)

0 0

100

200 N

300

400

FIG. 12. (Color online) (a) The average absolute writhe of (i) linear FENE chains in a melt (squares) and (ii) their PPs (diamonds) (the inset shows the corresponding double logarithmic plot). The black curve is the predicted scaling for individual semiflexible chains, cf. Eq. (26). We notice that for N > 80, |W | > 1. The dotted black curve is the scaling for equilateral RWs, Eq. (6), which much deviates from that of the flexible FENE chains and their PPs. (b) Same as above for the squared writhe. Mean-squared writhe of linear FENE chains (squares) and their PPs (diamonds). The black line shows the scaling for semiflexible chains, Eq. (28). The dotted black line shows the scaling for equilateral RWs, Eq. (6), for comparison.

approximated by Eq. (4). Thus, for an individual linear FENE chain embedded in a melt, which corresponds to a semiflexible chain of κ ≈ 2.34, we have (for N > 2) |W | ≈ 0.16N

2

4

〈Z〉

6

8

10

FIG. 13. The mean absolute writhe of a chain vs the average number of kinks per PP. Interestingly, the writhe of the individual chain in a melt seems to be related to the number of kinks in a multichain system, connecting thus local and global entanglement properties. Because the relationship is bijective, there is a one-to-one correspondence, which seems linear at first glance but is expected to be better described by Eq. (27) for large Z.

1

〈 WPP 〉

0 0

400

2

2

〈W 〉 60

300

1/2

+ 0.38N

−1/2

− 0.5.

(26)

This is in good agreement with the measured data shown in Fig. 12(a). In the same figure we show data for the mean absolute writhe of the corresponding PPs. It is interesting to notice that the average writhe in a dense system of flexible chains with excluded volume fits the general scaling of that of a WLC without excluded volume. Recall that the writhe is a measure of global self-entanglement (or complexity) of a fixed configuration of one chain. This suggests that an individual chain in the melt, on average,

assumes a similar configuration as a semiflexible chain in the vacuum with the stiffness parameter defined by the chain in the melt. Notice that this does not imply any relation of the two systems with respect to entanglements (kinks). Indeed, the FENE chains in a melt are entangled with each other, but chains in the vacuum are not entangled with others. The effect of the presence of other chains is intrinsically captured by the stiffness parameter κ ≈ 2.34, which determines the writhe of the chains in a melt. Moreover, the lp values suggest that the FENE chains of length N behave like random walks of length N/4, also supported by our data shown in Fig. 12(a). The writhe and the number of kinks in a chain are not related in general, since a chain (in the original state) with Z = 0 (in its reduced state) may have the same writhe with a chain with Z = 0. However, in a system for which we know that Z = 0, it makes sense to examine if there exists a relation between Z and |W |. Figure 13 shows the scaling of the mean absolute writhe of a chain with respect to the average number of kinks per chain for the system under study. Combining Eqs. (25) and (26) we see that, for N > 40, for linear FENE chains in a melt |W | and Z should be related as follows: |W | ≈ 1.25 (Z − 0.68)0.5 + 0.05 (Z − 0.68)−0.5 − 0.5.

(27)

Notice that Eq. (27) is based on the linear scaling of Z (for N > 40) and on Eq. (26). The linear scaling of Z has been confirmed by many studies [17,19,70] and Eq. (26) follows the form derived analytically by Kholodenko and Vilgis. This implies that, for this system, local and global entanglement properties of the chains may be related. We note that a relationship between the number of kinks in a system of freely jointed chains of tangent hard spheres and the probability of knotting has been proposed. Specifically, it is conjectured that the population of entanglements and knots follow the same

062604-10

WRITHE AND MUTUAL ENTANGLEMENT COMBINE TO . . .

W 2 ≈ 0.01N 1.18 .

(28)

This is captured by the data shown in Fig. 12(b) for the mean-squared writhe of a polymer chain. In the same figure we show data for the mean-squared writhe of the corresponding PPs. Notice that W 2 = Var(W ), since W = 0. The black curve shows the scaling of the mean-squared withe of FENE chains from Eq. (28) and the dotted black line shows the scaling of the corresponding equilateral random walks. Again, the values of the polymer chains are much smaller than those of random walks, as is now expected. From the variance of W , we can compute the error of its sample mean, erW . For a sample size of C melt configurations of M chains each, erW = √ 0.59 2 W /CM = 0.1 N / CM. Upon analyzing C = 100 independent configurations with M = 100 chains of length N < 400, the error erW < 0.004 is small compared to the reported values of W . C. The writhe of the primitive path

For a melt of ring polymers, if two chains are linked, the same must be true for the two corresponding PPs, if selfcrossings are not allowed. Even the link type of the PPs must be the same as that of the closed chains and consequently, their linking number is the same. Similarly, the knot type of both chains is the same as the knot types of their PP. But, the conformation differs significantly between a chain with N − 1 steps and its PP. The PP, as it is obtained by the Z1 algorithm, also is a polygonal chain, but with a reduced number of steps, Z + 1, and an increased average edge length. Even in the case of ring polymers, the writhe of each chain changes. In the case of linear polymers, both the linking number and the writhe of the chains will change continuously under the deformation of the chains. We note, however, that the effect of the reduction may differ for each measure. More precisely, the reduction respects the entanglements (kinks), which have an important impact on the linking integral of the two chains, but each chain becomes locally linear, which may have an important impact on the writhe of each chain. Numerical results [72] show that the linking integral of two chains is almost the same before and after the reduction. The writhe of the PP is a quantity that characterizes the global geometrical and topological complexity of the PP. It is therefore of particular interest to compare it to that of the original chain and to that of a random coil. Moreover, the writhe of the PP in addition to Z could provide further information on the nature of the kinks in a chain. For example, let us consider a configuration of a reduced chain with Z = 0 but whose kinks correspond to small bending angles. Its writhe will be approximately zero. If the bending angles of the kinks are large, as is usually the case for knotted arcs, then its writhe will be larger (see Fig. 1 for an illustrative example). Thus, the writhe of the PP could provide information about the nature of the kinks and the so-called persistent entanglements [69].

0

−1

2

log10 〈 |WPP| 〉 or 〈 WPP 〉

scaling laws at all volume fractions [33,38]. Using Eq. (27) we can estimate Z from writhe or the inverse. Thus, for this system, we can compute Ne estimators involving Z by computing the writhe of only a subcollection of chains. For the mean-squared writhe, following the previous discussion (Sec. II B1), for a FENE melt we have

PHYSICAL REVIEW E 88, 062604 (2013)

−2

−3 log 〈 |W 10

|〉

PP 2 log10〈 WPP 〉

−4

fit to N45 −5 1

1.5

2 log10N

2.5

3

FIG. 14. (Color online) Double-logarithmic plot of the mean absolute writhe and of the mean-squared writhe of the PPs. The different scaling with respect to N appears as a crossover (doubling slope) at about N ≈ 45.

Figure 12 shows the scaling of the mean absolute and the mean-squared writhe of a PP as a function of N and Fig. 14 shows the corresponding double logarithmic plots. Both quantities show a crossover at N ≈ 45. A crossover at N ≈ 45 appeared also for the scaling of Z. Thus, one should expect that this would also affect the writhe of the PPs. For N 45, the data are fitted to the function |WPP | = 0.006N 0.8 − 0.13, 2 = 0.00007N 1.56 − 0.02. WPP

(29)

We observe that the writhe of the PP is smaller than the writhe of the original chains. The normalized mean absolute difference between the writhe of the original and reduced chains, |W| = (|W − WPP |)/|W | is shown in Fig. 15(a). Figure 15(b) shows the corresponding double logarithmic plot. There might be a crossover at N ≈ 45 that is related to the previously mentioned crossover of |WPP | at the same N . Clearly, there is a crossover at N ≈ 80, where the relative difference decreases at a faster rate. Note that for N 80, |W | 1 which suggests that the chains of that length on average contain knots. Moreover, our estimate of Ne ≈ 80 provides further support for the entanglement of the chains. This crossover indicates that once the chains are entangled, there is a larger portion of the writhe of the original chains that remains in the PP. This transition could also be related to a change in the nature of the kinks with an increased presence of those with larger bending angles and thus to the presence of persistent entanglements. Edwards proposed that the PP behaves as a random coil [1]. From this viewpoint, the PP is also characterized by some persistence length that we may evaluate. One possible approach to estimating lp for the PP is to inspect the squared 2 end-to-end Ree values and compare these values with the formula for the WLC with L = Z + 1 segments of identical length (Appendix A). This yields a dimensionless lp for the PP and dimensionless κ via Eq. (A3). Using this method, we evaluate κ at each length. Indeed, for N = 10 and N = 20, the

062604-11

¨ E. PANAGIOTOU, M. KROGER, AND K. C. MILLETT

PHYSICAL REVIEW E 88, 062604 (2013)

in terms of the length scale over which orientation correlations are lost. Note that the bending angles might be actually larger than those of a FENE chain with excluded volume. Then, for this average κ, and for N = Z + 2, Eq. (26) gives different values for |WPP |. The data for the PP are best fitted to a function of the form

1

0.9

|WPP | ≈ 0.05 (Z + 2)1.26 − 0.36.

0.8

100

200 N

300

400

0.02 fit to N < 45 45< fit to N < 85 fit to N > 85 log10〈 |ΔW| 〉

0

log10 〈 |ΔW| 〉

−0.02 −0.04

2 From this analysis of |WPP | and WPP , we see that the PP cannot be modeled by semiflexible chains. A reason why one might expect a different scaling for the PP is because, at least for the data under consideration, the number of steps in a PP, as defined by Z is very small and may not be comparable to the data presented in Sec. II B1 which concern chains of length N 10. In fact, for N 400, we get Z + 2 10. By generating equilateral random walks of length N 10, the best fits of the mean absolute writhe and the mean-squared writhe are

|WRW | ≈ 0.2N 0.62 − 0.31, 2

WRW ≈ 0.01N 1.79 − 0.04,

−0.06 −0.08

(b)

−0.12 1

1.5

2 log N

2.5

3

10

FIG. 15. (Color online) (a) The normalized mean absolute difference of the writhe between the original and reduced chains, |W| = |W − WPP |/|W |. (b) Double logarithmic representation of the same data reveals moderate changes in slope at about N = 45 and N = 80.

reduced chains are in general straight rods, since there are no entanglements, and lp → ∞, as expected for very stiff chains. For N > 20 the values of lp result, via Eq. (A3), in values of κ that clearly indicate that the PPs are not random walks. However, as N increases, κ decreases, thus we cannot exclude the possibility that the PPs are well described by WLC’s with κ → 0 (random walks) as N → ∞. For all molecular weights observed in this study, the values of the writhe of the PP are small, consistent with what one would expect for a random coil of that length, i.e., with Z + 1 edges. In order to compare the behavior of the PPs with that of semiflexible chains, we will compare their writhes. To do this, we make the following approximations: first, we fix the stiffness parameter equal to its average value over all molecular weights; second, we let the number of steps of the PPs equal to Z + 1 for all PPs that correspond to original chains of length N ; and, third, we let the edge length of a PP to be equal to Ne for all PPs. For our data, the average stiffness of the PPs is κ ≈ 6.9. This is clearly a value that differs from that of the FENE chains or that of random walks. It indicates that the PP is much stiffer

(32) (33)

respectively, differing from those for N 10. These are shown with the dotted black curve in Figs. 16 and 17, respectively. We note that the writhe of the PPs becomes larger than the writhe of the RWs for Z + 2 > 5, which corresponds to the original chains of length N > 150. This suggests that the writhe of the PPs may be better compared to that of RWs of more than Z + 1 steps. The green lines in Figs. 16 and 17 show the mean 〈 |WPP| 〉 1.26

0.6

0.05 (〈 Z 〉 +2) (W )

0.4

(W

−0.36

RW 〈 Z 〉+2

〈 |WPP| 〉

−0.1

)

1.2

RW (〈 Z 〉−1)

0

0.2

−0.5 −1

0 −0.2

| 〉)

(a)

0.75 0

(30)

Similarly, for κ ≈ 6.9, the data of the mean-squared writhe are best fitted to the function 2

Z + 2 3.21 WPP ≈ 0.16 − 0.07. (31) κ

0.85

−1.5

Log(〈 |W

〈 |ΔW| 〉

0.95

−2.5

−2

−3 −3.5

−0.4 2

−4 0.2

4

6 〈 Z〉 +2

0.4

0.6 0.8 Log(〈 Z 〉 +2)

8

1

10

FIG. 16. (Color online) The mean absolute writhe of the primitive path as a function of the number of segments in a PP. The black curve shows the best fit for the mean absolute writhe of the PP, Eq. (30), and the dotted black curve shows the writhe of RWs of the same number of steps [Eq. (32)], i.e., Z + 1. We notice that the mean absolute writhe of the PPs is not that of RWs of Z + 1 edges. The inset shows the same data in double logarithmic plot.

062604-12

WRITHE AND MUTUAL ENTANGLEMENT COMBINE TO . . .

1.5 1

PP

PP

3.21

0.16 (〈 Z 〉+2)

0.5

− 0.07

(W2 ) RW 〈 Z 〉+2 2 (WRW)(〈 Z 〉−1)1.2

0.45

0 0

−0.5

−1

−1

0.35

Log(〈 W

−2

−1.5

0.3 −3 −4

−2 −2.5 2

0.4

〉)

〈 W2 〉

0.5

0.55

〈 W2 〉

〈 |We| 〉

2

PHYSICAL REVIEW E 88, 062604 (2013)

−5 0.2

4

0.25 0.4

6 〈Z〉 +2

0.6 0.8 Log(〈Z〉 +2)

1

8

0.2 0

10

FIG. 17. (Color online) The mean-squared writhe of the primitive path as a function of the number of segments in a PP. The black curve shows the best fit for the mean-squared writhe of the PP [Eq. (31)] and the dotted black curve shows the mean-squared writhe of RWs of the same number of steps [Eq. (33)], i.e., Z + 1. We notice that the mean-squared writhe of the PPs is not that of RWs of Z + 1 edges. The inset shows the same data in double logarithmic plot.

absolute and the mean-squared writhe of equilateral random walks of (Z − 1)1.2 vertices for comparison. D. The writhe of an entanglement strand

The entanglement strand, a part of the polymer chain of Ne monomers, is essential in the tube model. It determines a length scale at which a crossover from Rouse to reptation dynamics occurs. Therefore, it is of particular interest to examine the conformational properties of the chains at the length scale of the entanglement strands. In this section, based on the method presented in Sec. III to estimate Ne , we derive semianalytic formulas for the mean absolute and the mean-squared writhe of an entanglement strand. These quantities are measured for the first time and are expected to provide information about the self-entanglement and the conformational complexity of the polymer chains at the length scale of entanglement strands. 1. The mean writhe of an entanglement strand in a chain

The analysis in Sec. III allows us to compute the mean writhe of an entanglement strand in a chain from Eq. (11) as Z+1 W (ei ) We = i=1 Z+1 W − W (PP) , (34) = Z+1 where W denotes the writhe of the original chain and W (PP) denotes the writhe of its PP. This formula for We is semianalytic. For its derivation the only approximation used is the one described by Eq. (10). Thus, by Eq. (34) we can compute We , using only the writhe of the original and reduced chains and the number of kinks, without having to define directly the exact locations of the entanglement strands in a chain. The entanglement strands are defined only indirectly

100

200 N

300

400

FIG. 18. The average absolute mean writhe of an entanglement strand in a chain over all chains in a melt, We = |We |. It approaches an asymptotic value different than zero, as expected for an average over a sample of random coils of the same length. This may be related to the variance of the length of the entanglement strands in a chain.

by using the Z1 reduced chain as the PP of a chain in a melt and from that computing the writhe of the PP. Note that the writhe of an entanglement strand in a chain can take positive or negative values with the same probability. Thus, taking its average over all entanglement strands in the same chain, i.e., We will be approximately zero for a sufficiently long chain. For moderate molecular weights, which are the most common in numerical studies, We may be nonzero because the number of entanglement strands in the chain, i.e., Z + 1, may be small. Also, We will take both positive and negative values with the same probability, thus the mean writhe of an entanglement strand in a chain, averaged over all chains, is zero. For this reason, we will be interested in the value of the absolute value of the mean writhe of an entanglement strand in a chain, averaged over all chains, |We |, that can be derived from Eq. (34). In the following we will denote |We | by We . Figure 18 shows the values of We for our systems of linear FENE chains in a melt. The data suggest that We reaches an asymptotic value of approximately 0.4. It is interesting to note that even though the longer chains contain more entanglement strands, their mean writhe does not vanish. 2. The mean-squared writhe of an entanglement strand in a chain

Since the mean writhe of an entanglement strand in a chain is approximately equal to zero for very long chains, one would prefer to study the mean absolute writhe of an entanglement strand in a chain, averaged over all chains. Unfortunately, this is very difficult to accomplish. Following the analysis presented in Sec. III, we can measure the average, over all chains, of the mean-squared writhe of an entanglement strand in a chain by using Eq. (16). Since We ≈ 0, We2 is the average variance of the writhe of an entanglement strand in a chain over all chains, that is, We2 ≈ Var(W (e)). We note that Eq. (16) gives a semianalytic formula for We2 ≈ Var(W (e)). So, again, we can compute the average variance of the writhe of an entanglement strand without defining the locations of

062604-13

¨ E. PANAGIOTOU, M. KROGER, AND K. C. MILLETT

PHYSICAL REVIEW E 88, 062604 (2013)

the entanglement strands in a chain by using only Z and the writhe of the original and reduced chains. Figure 10 shows the values of We2 for our data. We observe that We2 seems to converge to an asymptotic value of approximately 2, which is consistent with the value of We2 = 1.88 for chains of length N = 80, as expected by our estimate of Ne ≈ 80, computed in Sec. IV B for this system. We observe that We2 > 1 for N > 95. This suggests the existence of entanglement strands with absolute writhe larger than one for long chains. Note that the chains of length N > 95 contain on average one entanglement strand of length Ne ≈ 80. This suggests that once entanglement strands are formed, there are probably some, on average, that contain knots. Note that knotted arcs at the length scale of Ne suggest the presence of self-entanglements in the reduced chains, since there is a large probability that no other chain interpenetrates. Interestingly, we arrive at the same result that was pointed out in Ref. [18]: Self-entanglement concerns local knotting or, more precisely, knotted arcs that are likely to occur at the length scale of the entanglement strands.

the writhe of a chain concerns a frozen initial configuration of a chain in a melt. Our numerical results show that the writhe of the Z1 reduced chains is significantly altered and that it is not comparable to that of semiflexible chains or random walks, indicating that the bending angles of the PPs are larger. From the analysis of Z and the difference of the writhe of the original and reduced chains, we observe two different crossovers in their scalings, at N ≈ 45, which indicates the presence of kinks, and at N ≈ 80, respectively, which indicates that the system is topologically entangled. This finding suggests a possible explanation for the discrepancies between the different Ne estimators. Finally, we provide a semianalytical expression for the mean and the mean-squared writhe of an entanglement strand, Eqs. (16) and (34). This measures the conformational complexity at the length scale of entanglement strands. Our numerical results on linear FENE chains in a melt suggest that for long chains the entanglement strands may contain knots. ACKNOWLEDGMENTS

This research was supported by a Swiss Government Scholarship (Reference No. 2011.0409).

VI. CONCLUSIONS

In this study, the writhe, a global measure of selfentanglement of a chain, and Z, the number of kinks in the PP network for a multichain polymer melt configuration, are used to define an estimator of Ne , the number of monomers in an entanglement strand, via Eq. (24). An advantage of this estimator is that it is valid for both open and closed chains in any PBC model. Moreover, it does not depend directly on the exact locations where the kinks occur, nor on the value of Lpp . We have applied our method to linear FENE chains in a melt in equilibrium conditions. Our estimate Ne ≈ 80 is in good agreement with values reported from experiments. This provides strong evidence that the combination of local and global entanglement measures can provide information that is relevant to the study of entanglement in polymers. By comparing our estimator with previous estimators, we observe that it converges faster than the S estimators. Another strength of this estimator is that it does not rely on a smooth set of data for various molecular weights as required by the M-kink estimator to unambiguously calculate numerical derivatives. In the course of developing the estimator we numerically studied the mean absolute and the mean-squared writhe of linear semiflexible chains. Our numerical results suggest a scaling similar to the analytical prediction of Kholodenko and Vilgis for semiflexible ring polymers, Eq. (4). Focusing on linear FENE chains in a melt in equilibrium conditions, our results suggest a relation of the form described by Eq. (26) for the mean absolute writhe. This result confirms that the polymer chains in a melt have characteristics similar to those of semiflexible chains in the vacuum with a stiffness parameter determined by the system. For our systems of linear FENE chains in a melt, we observe that Z and the writhe of the chains are related by Eq. (27). Although this is not a general result, it is of interest since, at first glance, one might expect these quantities to be unrelated because they capture different entanglement information. Also, the average number of kinks per chain, Z, is computed from the Z1 reduced chains, while

APPENDIX A: WORMLIKE CHAINS

Consider a wormlike chain (WLC), a connected linear string of N − 1 segment unit vectors ui = ri+1 − ri that connect N 1 nodes located at ri . With cos θi = ui · ui+1 we may call θi ∈ [0,π ] a bending angle between segments i and i + 1. The Hamiltonian of the discrete WLC is H = −κkB T

N−2

cos θi ,

(A1)

i=1

with dimensionless bending stiffness κ. Within the canonical ensemble the dimensionless persistence length, lp , characterizing the orientational correlation of bonds, |i − j | , (A2) ui · uj = exp − lp can be calculated analytically in terms of κ, lp = −

1 . ln[coth(κ) − 1/κ]

(A3)

At κ 1 this rapidly approaches lp ≈ κ − 1/2 and lp = 1 for κ ≈ 1.21. The Kuhn length can be derived from the persistence length as lk ≈ 2lp . The mean-squared end-to-end distance of the WLC is analytically obtained from Eq. (A2), lp (A4) R 2 = 2lp L 1 − (1 − e−L/ lp ) , L where L ≡ N − 1. The equilateral random walk exhibiting R 2 = L is recovered from Eq. (A4) for L lp = 1/2 (or κ ≈ 0.4106). The opposite extreme, a stiff chain exhibiting R 2 = L2 is recovered for L lp → ∞ (i.e., large κ 1). WLCs with the correct statistics of the canonical ensemble can be grown segmentwise via Monte Carlo using random numbers x equally distributed over the interval [0,1] as follows cos θi = κ −1 ln(2x sinh κ). These bending angles give

062604-14

WRITHE AND MUTUAL ENTANGLEMENT COMBINE TO . . .

rise to the probability distribution p(θ ) ∼ exp(κ cos θ ) sin θ . π Employing 0 p(θ )dθ = 1 one arrives at p(θ ) =

κ exp(κ cos θ ) sin(θ ) . 2 sinh(κ)

(A5)

APPENDIX B: THE WRITHE OF A CHAIN WITH RESPECT TO ITS ENTANGLEMENT STRANDS

Let us consider a polymer chain, I , with parametrization γ , formed by Z + 1 entanglement strands, say ei ,i = 1, . . . ,Z + 1, with parametrizations γi ,i = 1, . . . ,Z + 1 respectively. Then the writhe of I can be expressed as (γ˙ (t),γ˙ (s),γ (t) − γ (s)) 1 dtds W (I ) = 2π [0,1]∗ [0,1]∗ |γ (t) − γ (s)|3 Z+1 1 (γ˙i (t),γ˙i (s),γi (t) − γi (s)) = dtds 2π i=1 [0,1]∗ [0,1]∗ |γi (t) − γi (s)|3 Z Z+1 1 + 2π i=1 j =i+1 [0,1] [0,1] × =

(γ˙i (t),γ˙j (s),γi (t) − γj (s)) dtds |γi (t) − γj (s)|3

Z+1 i=1

W (ei ) + 2

Z Z+1

L(ei ,ej ),

PHYSICAL REVIEW E 88, 062604 (2013)

Consider the second term in the right-hand side of (C1). First, recall that W (ei ),W (ej ) are the writhe of the i-th and j -th entanglement strands of a chain, respectively. As N → ∞, Ne is expected to approach an asymptotic value [17]. Thus, for large-enough N , Z, and Ne are independent random variables. The writhe of an entanglement strand depends only on Ne , and thus for large N , it is also independent of Z. So, in the following we make the approximation W (ei )W (ej ) 1 ≈ W (ei )W (ej ) . (C2) Z+1 Z+1 Next we notice that each entanglement strand is a random polymer chain, independent of the other entanglement strands, so the terms W (ei ) and W (ej ) are independent random variables, and, thus, W (ei )W (ej ) = W (ei )W (ej ). But W (ei ) is independent of the index i, thus W (ei ) = W (ej ) = W (e). Since each entanglement strand in the space of configurations can have positive or negative writhe with the same probability, W (ei ) = W (ej ) = W (e) = 0. Thus, the second term in the right-hand side of (C1) vanishes, and Eq. (C1) becomes [W (I ) − W (PP(I ))]2 2 . (C3) We ≈ Z+1 APPENDIX D: DISTRIBUTION OF Ne

(B1)

i=1 j =i+1

where W (ei ) denotes the writhe of the entanglement strand ei and L(ei ,ej ) denotes the Gauss linking number of the entanglement strands i and j . APPENDIX C: THE MEAN-SQUARED WRITHE OF AN ENTANGLEMENT STRAND

The mean-squared writhe of an entanglement strand in a chain averaged over all chains in a melt is given by Eq. (15), namely W (ei )W (ej ) (W (I ) − W (PP(I )))2 2 −2 . We = Z+1 Z+1 i